International
Tables for Crystallography Volume D Physical properties of crystals Edited by A. Authier © International Union of Crystallography 2013 |
International Tables for Crystallography (2013). Vol. D, ch. 1.7, pp. 186-188
Section 1.7.3.1.1. Index surface and electric field vectors^{a}Institut Néel CNRS Université Joseph Fourier, 25 rue des Martyrs, BP 166, 38042 Grenoble Cedex 9, France, and ^{b}Laboratoire de Photonique Quantique et Moléculaire, Ecole Normale Supérieure de Cachan, 61 Avenue du Président Wilson, 94235 Cachan, France |
The relations between the different field vectors relative to a propagating electromagnetic wave are obtained from the constitutive relations of the medium and from Maxwell equations.
In the case of a non-magnetic and non-conducting medium, Maxwell equations lead to the following wave propagation equation for the Fourier component at the circular frequency ω defined by (1.7.2.15) and (1.7.2.16) (Butcher & Cotter, 1990):where , λ is the wavelength and c is the velocity of light in a vacuum; is the free-space permeability, E(ω) is the electric field vector and P(ω) is the polarization vector.
In the linear regime, , where _{0} is the free-space permittivity and χ^{(1)}(ω) is the first-order electric susceptibility tensor. Then (1.7.3.1) becomes is the dielectric tensor. In the general case, is a complex quantity i.e. . For the following, we consider a medium for which the losses are small (); it is one of the necessary characteristics of an efficient nonlinear medium. In this case, the dielectric tensor is real: .
The plane wave is a solution of equation (1.7.3.2):() is the orthonormal frame linked to the wave, where Z is along the direction of propagation.
We consider a linearly polarized wave so that the unit vector e of the electric field is real (), contained in the XZ or YZ planes.
is the scalar complex amplitude of the electric field where is the phase, and . In the linear regime, the amplitude of the electric field varies with Z only if there is absorption.
k is the modulus of the wavevector, real in a lossless medium: corresponds to forward propagation along Z, and to backward propagation. We consider that the plane wave propagates in an anisotropic medium, so there are two possible wavevectors, k^{+} and k^{−}, for a given direction of propagation of unit vector u:() are the spherical coordinates of the direction of the unit wavevector u in the optical frame; () is the optical frame defined in Section 1.7.2.
The spherical coordinates are related to the Cartesian coordinates () byThe refractive indices , , real in the case of a lossless medium, are the two solutions of the Fresnel equation (Yao & Fahlen, 1984):n_{x}(ω), n_{y}(ω) and n_{z}(ω) are the principal refractive indices of the index ellipsoid at the circular frequency ω.
Equation (1.7.3.6) describes a double-sheeted three-dimensional surface: for a direction of propagation u the distances from the origin of the optical frame to the sheets (+) and (−) correspond to the roots n^{+} and n^{−}. This surface is called the index surface or the wavevector surface. The quantity () or () is the birefringency. The waves (+) and (−) have the phase velocities and , respectively.
Equation (1.7.3.6) and its dispersion in frequency are often used in nonlinear optics, in particular for the calculation of the phase-matching directions which will be defined later. In the regions of transparency of the crystal, the frequency law is well described by a Sellmeier equation, which is the case for normal dispersion where the refractive indices increase with frequency (Hadni, 1967):If ω_{i}_{ }or ω_{j} are near an absorption peak, even weak, n^{±}(ω_{i}) can be greater than n^{±}(ω_{j}); this is called abnormal dispersion.
The dielectric displacements , the electric fields , the energy flux given by the Poynting vector and the collinear wavevectors are coplanar and define the orthogonal vibration planes (Shuvalov, 1981). Because of anisotropy, and , and hence and , are non-collinear in the general case as shown in Fig. 1.7.3.1: the walk-off angles, also termed double-refraction angles, are different in the general case; , , and are the unit vectors associated with , , and , respectively. We shall see later that the efficiency of a nonlinear interaction is strongly conditioned by k, E and ρ, which only depend on χ^{(1)}(ω), that is to say on the linear optical properties.
The directions S^{+} and S^{−} are the directions normal to the sheets (+) and (−) of the index surface at the points n^{+} and n^{−}.
For a plane wave, the time-average Poynting vector is (Yariv & Yeh, 2002) is the energy flow , which is a power per unit area i.e. the intensity, where is the energy of the photon and are the photons flows. ρ^{±}(ω) is the angle between S^{±} and u; it is detailed later on.
The unit electric field vectors e^{+} and e^{−}are calculated from the propagation equation projected on the three axes of the optical frame. We obtain, for each wave, three equations which relate the three components () to the unit wavevector components () (Shuvalov, 1981):with
The vibration planes relative to the eigen polarization modes are called the neutral vibration planes associated with u: an incident linearly polarized wave with a vibration plane parallel to or is refracted inside the crystal without depolarization, that is to say in a linearly polarized wave, e^{+} or e^{–}, respectively. For any other incident polarization the wave is refracted in the two waves e^{+} and e^{−}, which propagate with the difference of phase .
The existence of equalities between the principal refractive indices determines the three optical classes: isotropic for the cubic system; uniaxial for the tetragonal, hexagonal and trigonal systems; and generally biaxial for the orthorhombic, monoclinic and triclinic systems [Nye (1957) and Sections 1.1.4.1 and 1.6.3.2 ].
References
Butcher, P. N. & Cotter, D. (1990). The elements of nonlinear optics. Cambridge series in modern optics. Cambridge University Press.Hadni, A. (1967). Essentials of modern physics applied to the study of the infrared. Oxford: Pergamon Press.
Nye, J. F. (1957). Physical properties of crystals. Oxford: Clarendon Press.
Shuvalov, L. A. (1981). Modern crystallography IV – Physical properties of crystals. Springer Series in solid-state sciences No. 37. Heidelberg: Springer Verlag.
Yao, J. Q. & Fahlen, T. S. (1984). Calculations of optimum phase match parameters for the biaxial crystal KTiOPO_{4}. J. Appl. Phys. 55, 65–68.
Yariv, A. & Yeh, P. (2002). Optical waves in crystals. New York: Wiley.